Presentation on theme: "If cannot bear such conditions…"— Presentation transcript:
1If cannot bear such conditions… Sub-topicsFailureDuctile and brittle fractureFracture toughnessFundamentals of fracture mechanics
2Failure Failure in structures leads to lost of properties and sometimes lost ofhuman lives.An oil tanker that fractured in a brittle manner by crack propagation around its girth. (Photography by Neal Boenzi. Reprinted with permission from The New York Times.)
3Types of fractureFracture is the separation of a body into two or more pieces in response to an imposed stress that is static and at temperatures that are low relative to the melting temperature of the material.
4Failure modesDuctile fracture is almost always preferred to brittle one.Highly ductile fracture inwhich the specimen necks down to a pointModerately ductile fracture after somenecking.Brittle fracture without anyplastic deformation.
5Ductile fracture Highly ductile fracture in which the specimen necks down to a point
6Cup-and-cone fracture in aluminum. Ductile fractureSmall cavity formationInitial necking.Coalescence ofcavities to form a crackCup-and-cone fracture in aluminum.CrackpropagationFinal shear fracture.
7Tough “ductile” fracture Ductile fracture is a much less seriousproblem in engineering materials sincefailure can be detected beforehand dueto observable plastic deformationprior to failure.Under uniaxial tensile force, afternecking, microvoids form andcoalesce to form crack, which thenpropagate in the direction normal tothe tensile axis.The crack then rapidly propagatethrough the periphery along the shearplane, leaving the cub andcone fracture.
8Microvoid formation, growth and coalescence • Microvoids are easily formed at inclusions, intermetallic or second-phase particles and grain boundaries.• Growth and coalescence of microvoids progress as the local applied load increases.Random planar arrayof particles acting asvoid initiatorsLinkage or coalescenceof these voids to form free fracture surface.Growth of voids to joineach other as the appliedstress increases.
9Ductile fracture of alloys If materials is stretched, it firstly deforms uniformly.Inclusions – stress concentrators
10Formation of microvoids from second phase particles 1) Decohesion at particle -matrix interface.2) Fracture of brittle particle3) Decohesion of an interface associated with shear deformation or grainboundary sliding.Fractured carbides aidingmicrovoid formation.Decohesion of carbide particlesfrom Ti matrix.
12Fractografic studies Scanning electron fractograph of ductile cast iron showing a transgranular fracture surface.Scanning electronfractograph showingan intergranularfracture surface.
13Nature of fracture: brittle Characteristic for ceramics and glassesDistinct characteristics of brittle fracture surfaces:1) The absence of gross plastic deformation.2) Grainy or Faceted texture.3) “River” marking or stress lines.
14Intergranular fracture • Intergranular failure isa moderate to low energybrittle fracture mode resultingfrom grain boundaryseparation or segregation ofembrittling particles orprecipitates.• Embrittling grainboundary particles areweakly bonded with thematrix, high free energyand unstable, which leads topreferential crackpropagation path.Intergranular fracture with and withoutmicrovoid coalescence
15Strength and toughness Resistance of a materialto plastic flowToughnessResistance of a materialto the propagationof a crackHow concerned should you be if you read in the paper that cracks have been detected in the pressure vessel of the nuclear reactor of the power station a few miles away?
16Testing for toughnessMeasuring the energyImpact testTear testThis type of test provides a comparison of the toughness of materials –however, it does not provide a way to express toughness as a material property (no true material property that is independent on size and shape of the test sample)
17Introduction to fracture mechanics The fracture strength of a solid material is a function of thecohesive forcesthat exist between atoms.surface energyunstrained interatomic spacingOn this basis, the theoretical cohesive strength of a brittle elastic solid has been estimated to be approximately E/10, where E is the modulusof elasticity.The experimental fracture strengths of most engineering materialsnormally lie between 10 and 1000 times below this theoretical value.Why?
18Cracks concentrate stress Stress concentrationCrack reduces the cross – section => increase in stressWhat will happen with tough material?Cracks concentrate stressFlaws are detriment to the fracture strength because an applied stress may be amplified or concentrated at the tip, the magnitude of this amplification depends on crack orientation and geometry.
21Stress concentrators the magnitude of this localized stress diminishes with distance away from the crack tipThe maximum stress at the crack tipSchematic stress profile along the line X–XA measure of the degree to which an external stress is amplified at the tip of a crackstress concentration factor
22Problem1. Consider a circular hole in a plate loaded in tension. When will material near the hole yield?2. A plate with a rectangular section500 mm by 15 mm carries a tensile load of 50kN.It is made of a ductile metal with a yield strength of 50 MPa.The plate contains an elliptical hole of length 100 mm and a minimum radius of 1 mm, oriented as shown in the diagram.What is(a) the nominal stress(b) The maximum stress in the plate?(c) Will the plate start to yield?(d) Will it collapse completely?
24Griffith theory of brittle fracture Inherent defects in brittlematerials lead to stressconcentration.If stress exceeds the cohesive strength of bonds, crack extension is possible.Thermodynamic criterion:There are two energies to be taken into account when a crack propagates:New surfaces should be created and a certain amount of energy must be provided to create them;Elastic strain energy stored in the stressed material is released during crack propagation.
25Theory of brittle fracture The stress required tocreate the new crack surfaceG ≥ 2γCritical stress for crack propagationThe strain energy release rate (G) is higher for higher loads and larger cracks.If the strain energy released exceeds a critical value,then the crack will grow spontaneously.For brittle materials, stress can be equal to the surface energy of the (two) new crack surfaces; in other words, in brittle materials, a crack will grow spontaneously if the strain energy released is equal to or greater than the energy required to grow the crack surface(s).The stability condition can be written aselastic energy released (G) = surface energy created (2γ)If the elastic energy release is less than the critical value,the crack will not grow.
26ProblemA relatively large plate of a glass is subjected to a tensile stress of 40 MPa. If the specific surface energy and modulus of elasticity for this glass are 0.3 J/m2 and 69 GPa, respectively,determine the maximum length of a surface flaw that is possible without fracture.
27Problem: Properties of SiAlON Ceramics Assume that an advanced ceramic, SiAlON (silicon aluminum oxynitride),has a tensile strength of 414 MPa.Let us assume that this value is for a flaw-free ceramic. (In practice, it is almost impossible to produce flaw-free ceramics.)A crack cm deep is observed before a SiAlON part is tested.The part unexpectedly fails at a stress of 3.5 MPa by propagation of the crack.Estimate the radius of the crack tip.
28basic modes of crack tip deformation K = (EG) 1/2critical stress for crack propagationKIC – the critical stress intensity in mode I fracture (plain strain)
29Fracture toughness Fracture toughness of a material is obtained by determiningthe ability of a material to withstand the load in the presence ofa sharp crack before failure.FT is a material property;Value is independent of the way it is measured;Can be used for designCrack propagates when the stress intensity factor exceeds a critical value.Y is a dimensionless parameter or function that depends on both crack and specimen sizes and geometries, as well as the manner of load application
30G≥ 2γ Energy release rate Irwin later modified the Griffith theory by replacing the term 2γ with the potential strain energy release rate GWhen a samples fractures, a new surface is created => necessary conditions for fracture – sufficient energy releaseG≥ 2γThe critical condition to which the crackpropagates to cause global failure is when this G value exceeds the critical valueIrwin showed that G is measurable and can be related to the stress intensity factor, K
32A plastic zone forms at the Process zoneA plastic zone forms at thecrack tip where the stresswould otherwise exceedthe yield strengthSize of process zone:
33Brittle “cleavage” fracture Materials of high yield strengthNear tip stress are very high =>tear the atomic bonds apart =>increase in the crack length results in increase in K, causing crack to accelerate
34Fracture toughness and design If the KIC value of material is known and the presence of a crack is allowed, we can then monitor the crack propagation during service prior to failure =>How long we can use the component before it fails.Brittle materials, for which appreciable plastic deformation is not possible in front of an advancing crack, have low KIc values and are vulnerable to catastrophic failure.Crack length necessaryfor fracture at a materialsyield strength
35Damage tolerance Critical crack lengths are a measure of the damage tolerance of a materialTough metals are able to containlarge cracks but still yield in apredictable, ductile, manner
36Fracture resistanceThe ability of a material to resist the growth of a crack depends on a large number of factors:Larger flaws reduce the permitted stress.The ability of a material to deform is critical.Increasing the rate of application of the load, such as that encountered in an impact test, typically reduces the fracture toughness of the material.Increasing the temperature normally increases the fracture toughness.
38Fracture toughness – modulus chart Values range from 0.01 – 100 MPa√m
39Transition crack length plotted on chart – values can range from near-atomic dimensions for ceramics to almost a meter for ductile metals
40Fail-Safe Design Yield-before-break Leak-before-break Requires that the crack willnot propagate even if thestress causes the part to yieldLeak-before-breakRequires that a crackjust large enough topenetrate both the innerand outer surface of thevessel is still stable
41Design using fracture mechanics wall stressConsider the thin-walled spherical tank of radius r and thickness t that may be used as a pressure vessel.One design of such a tank calls for yielding of the wall material prior to failure as a result of the formation of a crack of critical size and its subsequent rapid propagation.Thus, plastic distortion of the wall may be observed and the pressure within the tank released before the occurrence of catastrophic failure.Consequently, materials having large critical crack lengths are desired.On the basis of this criterion, rank the metal alloys listed in Table, as to critical crack size, from longest to shortest.
42Design process – yield-before-fracture Requirement:The stresses are everywhere less that required to make a crack of critical length to propagate.BUT!!! It is not safe…Requirement:Crack should not propagate even if the stress is sufficient to cause general yield – for then the vessel will deform stably in a way that can be detected.≤Tolerable crack size
43Design problem - leak-before-break An alternative design that is also often utilized with pressure vessels is termed leak-before-break. Using principles of fracture mechanics, allowance is made for the growth of a crack through the thickness of the vessel wall prior to the occurrence of rapid crack propagation. Thus, the crack will completely penetrate the wall without catastrophic failure, allowing for its detection by the leaking of pressurized fluid.With this criterion the critical crack length ac (i.e., one-half of the total internal crack length) is taken to be equal to the pressure vessel thickness t.2a = tUsing this criterion, rank the metal alloys in Table as to the maximum allowable pressure.≤
44Forensic fracture case K1c of the tank material measured to be 45 MPa√m10 mm crack found in longitudinal weldStress based onmaximum designpressureStress at which a plate with the given K1c will fail with a 10 mm crack
45Design of a ceramic support Determine the minimum allowable thickness for a 7.5 cm wide plate made of sialon (SiAlON or silicon aluminumoxynitride) that has a fracture toughness of 9.9 Mpa m1/2.The plate must withstand a tensile load of N.The part will be non-destructively tested to ensure that no flaws are present that might cause failure.The minimum allowable thickness of the part will depend on the minimum flaw size that can be determined by the available testing technique.Assume that three non-destructive testing techniques are available:X-ray radiography can detect flaws larger than 0.05 cm;gamma-ray radiography can detect flaws larger than 0.02 cm; and ultrasonic inspection can detect flaws larger than cm.Assume that the geometry factor f = 1.0 for all flaws.
46Ductile-to-Brittle transition At low temperatures some metals and all polymers become brittleAs temperatures decrease, yield strengths of most materials increase leading to a reduction in the plastic zone sizeOnly metals with an FCC structure remain ductile at the lowest temperaturesThe ductile to brittle transition temperature is the temperature at which the failure mode of a material changes from ductile to brittle fracture.
47Ductile to brittle transition behaviour Some metals and polymers experience ductile-to-brittle transition behaviour when subjected to decreasing temperature, resulting from a strong yield stress dependence on temperature.Metals possess limitedslip systems available at low temperature, minimising the plastic deformation during thefracture process.Increasing temperatureallows more slip systems tooperate, yielding generalplastic deformation to occurprior to failure.
48When ductile turn to brittle The criterion for a material to change its fracture behaviour from ductile to brittle mode is when the yield stress at the observed temperature is larger than the stress necessary for the growth of the micro-crack indicated in the Griffith theoryThe criterion for ductile to brittle transition is when the term on the left hand side is greater than the right hand side.τ is the lattice resistance to dislocation movementk’ is a parameter related to the release of dislocation into a pile-upD is the grain diameter (associated with slip length).G is the shear modulusβ is a constant depending on the stress system
49Why don’t some materials undergo transition? Unlike steel, aluminium does not undergo a ductile-brittle transition. The reason can be explained in terms of their crystal structure.The yield stress of steel is temperature sensitive because of its BCC structure. At low temperatures it is more difficult for the dislocations to move (they require a degree of diffusion to move due to the non-close packed nature of the slip planes) and therefore plastic deformation becomes more difficult. The effect of this is to increase the yield stress at low temperatures.Aluminium has a FCC structure, this means that it has lots of easily operated close-packed slip systems operating at low temperatures. As a result its yield strength is not temperature sensitive and aluminium remains ductile to low temperatures.
50Bad luck of “Titanic”The sinking of the “Titanic” was caused primarily by the brittleness of the steel used to construct the hull of the ship.In the icy water of the Atlantic, the steel was below the ductile to brittle transition temperature.
51Factors affecting modes of fracture The yield stress of steel is temperature sensitive. The fracture stress remains relatively constant with temperature.At room temperature steel is a ductile material, this means that it will undergo plastic deformation before fracture i.e. the yield strength of the material is less than the fracture stress.At low temperatures the yield stress of steel increases, when the yield stress increases above the fracture stress the material will undergo aductile-to-brittle transition.
52The Strength-Toughness trade-off Increasing the yieldstrength of a metaldecreasing the sizeof the plastic zonesurrounding a crack –this leads to decreasedtoughness
53Metallurgical aspect of fracture • Microstructure in metallic materials are highly complex.• Various microstructural features affect how the materials fractureThere are microstructuralfeatures that can play a role in determining the fracture path, the most important are• High strength materials usually possess several microstructural features in order to optimise mechanical properties byinfluencing deformation behaviour /fracture paths.